 Molar mass distribution

In linear polymers the individual polymer chains rarely have exactly the same degree of polymerization and molar mass, and there is always a distribution around an average value. The molar mass distribution (or molecular weight distribution) in a polymer describes the relationship between the number of moles of each polymer species (N_{i}) and the molar mass (M_{i}) of that species. ^{[1]} The molar mass distribution of a polymer may be modified by polymer fractionation.
Contents
Definition of molar mass averages
Different average values can be defined depending on the statistical method that is applied. The weighted mean can be taken with the weight fraction, the mole fraction or the volume fraction:
 Number average molar mass or M_{n}
 Weight average molar mass or M_{w}
 Viscosity average molar mass or M_{v}
 Z average molar mass or M_{z}
^{[2]}
Here a is the exponent in the MarkHouwink equation that relates the intrinsic viscosity to molar mass.
Measurement
These different definitions have true physical meaning because different techniques in physical polymer chemistry often measure just one of them. For instance, osmometry measures number average molar mass and smallangle laser light scattering measures weight average molar mass. M_{v} is obtained from viscosimetry and M_{z} by sedimentation in an analytical ultracentrifuge. The quantity a in the expression for the viscosity average molar mass varies from 0.5 to 0.8 and depends on the interaction between solvent and polymer in a dilute solution. In a typical distribution curve, the average values are related to each other as follows: M_{n} < M_{v} < M_{w} < M_{z}. Polydispersity of a sample is defined as M_{w} divided by M_{n} and gives an indication just how narrow a distribution is.^{[2]}
The most common technique for measuring molecular weight used in modern times is a variant of highpressure liquid chromatography (HPLC) known by the interchangeable terms of size exclusion chromatography (SEC) and gel permeation chromatography (GPC). These techniques involve forcing a polymer solution through a matrix of crosslinked polymer particles at a pressure of up to several thousand psi. The limited accessibility of stationary phase pore volume for the polymer molecules results in shorter elution times for highmolecularweight species. The use of low polydispersity standards allows the user to correlate retention time with molecular weight, although the actual correlation is with the Hydrodynamic volume. If the relationship between molar mass and the hydrodynamic volume changes (i.e., the polymer is not exactly the same shape as the standard) then the calibration for mass is in error.
The most common detectors used for size exclusion chromatography include online methods similar to the bench methods used above. By far the most common is the differential refractive index detector that measures the change in refractive index of the solvent. This detector is concentrationsensitive and very molecularweightinsensitive, so it is ideal for a singledetector GPC system, as it allows the generation of mass v's molecular weight curves. Less common but more accurate and reliable is a molecularweightsensitive detector using multiangle laserlight scattering  see Static Light Scattering. These detectors directly measure the molecular weight of the polymer and are most often used in conjunction with differental refractive index detectors. A further alternative is either lowangle light scattering, which uses a single low angle to determine the molar mass, or RightAngleLight Laser scattering in combination with a viscometer, although this latter technique does not give an absolute measure of molar mass but one relative to the structural model used.
The molar mass distribution of a polymer sample depends on factors such as chemical kinetics and workup procedure. Ideal stepgrowth polymerization gives a polymer with polydispersity of 2. Ideal living polymerization results in a polydispersity of 1. By dissolving a polymer an insoluble high molar mass fraction may be filtered off resulting in a large reduction in M_{w} and a small reduction in M_{n} thus reducing polydispersity.
Number average molecular weight
The number average molecular weight is a way of determining the molecular weight of a polymer. Polymer molecules, even ones of the same type, come in different sizes (chain lengths, for linear polymers), so the average molecular weight will depend on the method of averaging. The number average molecular weight is the ordinary arithmetic mean or average of the molecular weights of the individual macromolecules. It is determined by measuring the molecular weight of n polymer molecules, summing the weights, and dividing by n.
The number average molecular weight of a polymer can be determined by gel permeation chromatography, viscometry via the (MarkHouwink equation), colligative methods such as vapor pressure osmometry, endgroup determination or proton NMR ^{[3]}.
An alternative measure of the molecular weight of a polymer is the weight average molecular weight. The ratio of the weight average to the number average is called the polydispersity index.
High NumberAverage Molecular Weight Polymers may be obtained only with a high fractional monomer conversion in the case of stepgrowth polymerization, as per the Carothers' equation.
Weight average molecular weight
The weight average molecular weight is a way of describing the molecular weight of a polymer. Polymer molecules, even if of the same type, come in different sizes (chain lengths, for linear polymers), so we have to take an average of some kind. For the weight average molecular weight, this is calculated by
where N_{i} is the number of molecules of molecular weight M_{i}.
If the weight average molecular weight is w, and one chooses a random monomer, then the polymer it belongs to will have a weight of w on average (for a homopolymer).
The weight average molecular weight can be determined by light scattering, small angle neutron scattering (SANS), Xray scattering, and sedimentation velocity.
An alternative measure of molecular weight for a polymer is the number average molecular weight; the ratio of the weight average to the number average is called the polydispersity index.
The weightaverage molecular weight, M_{w}, is also related to the fractional monomer conversion, p, in stepgrowth polymerization as per Carothers' equation:
 , where M_{o} is the molecular weight of the repeating unit.
See also
References
 ^ I. Katime "Química Física Macromolecular". Servicio Editorial de la Universidad del País Vasco. Bilbao
 ^ ^{a} ^{b} R.J. Young and P.A. Lovell, Introduction to Polymers, 1991
 ^ Polymer Molecular Weight Analysis by 1H NMR Spectroscopy Josephat U. Izunobi and Clement L. Higginbotham J. Chem. Educ., 2011, 88 (8), pp 1098–1104 doi:10.1021/ed100461v
Categories:
Wikimedia Foundation. 2010.
Look at other dictionaries:
Mass distribution — For other uses, see Weight distribution. Mass distribution is a term used in physics and mechanics and describes the spatial distribution of mass within a solid body. In principle, it is relevant also for gases or liquids, but on earth their mass … Wikipedia
Molar mass — Formula mass redirects here. It is not to be confused with Mass formula. Molar mass, symbol M,[1] is a physical property of a given substance (chemical element or chemical compound), namely its mass per amount of substance.[2] The base SI unit… … Wikipedia
Absolute molar mass — is a process to determine the characteristics of molecules. TOC History The first absolute measurements (i.e. made without reference to standards) were based on fundamental physical characteristics and their relation to the molar mass. The most… … Wikipedia
Distribution constant — The distribution constant (or partition ratio), is the equilibrium constant for the distribution of an analyte in two immiscible solvents.[1] For a particular solvent, it is equal to the ratio of its molar concentration in the stationary phase to … Wikipedia
Molecular mass — This article is about the mass of a single molecule. For the mass of a substance commonly used in basic stoichiometric calculations, see Molar mass. Assuming hydrogen and oxygen are standard weights in this image (as opposed to deuterium oxide)… … Wikipedia
Maxwell–Boltzmann distribution — Maxwell–Boltzmann Probability density function Cumulative distribution function parameters … Wikipedia
Monoisotopic mass — This article is about the mass spectrometry term. For a list of monoisotopic elements, see stable isotope. The monoisotopic mass is the sum of the masses of the atoms in a molecule using the unbound, ground state, rest mass of the principal (most … Wikipedia
Sizeexclusion chromatography — Equipment for running size exclusion chromatography. The buffer is pumped through the column (right) by a computer controlled device Acronym SEC Classification Chromatography Analytes … Wikipedia
Matrixassisted laser desorption/ionization — MALDI TOF mass spectrometer Matrix assisted laser desorption/ionization (MALDI) is a soft ionization technique used in mass spectrometry, allowing the analysis of biomolecules (biopolymers such as DNA, proteins, peptides and sugars) and large… … Wikipedia
Chemical kinetics — Reaction rate tends to increase with concentration a phenomenon explained by collision theory. Chemical kinetics, also known as reaction kinetics, is the study of rates of chemical processes. Chemical kinetics includes investigations of how… … Wikipedia